Drawing (manufacturing)

Drawing is a metalworking process which uses tensile forces to stretch metal, glass, or plastic. As the metal is drawn (pulled), it stretches thinner, into a desired shape and thickness. Drawing is classified in two types: sheet metal drawing and wire, bar, and tube drawing. The specific definition for sheet metal drawing is that it involves plastic deformation over a curved axis. For wire, bar, and tube drawing, the starting stock is drawn through a die to reduce its diameter and increase its length. Drawing is usually done at room temperature, thus classified a cold working process, however it may be performed at elevated temperatures to hot work large wires, rods or hollow sections in order to reduce forces. 
Drawing differs from rolling in that the pressure of drawing is not transmitted through the turning action of the mill but instead depends on force applied locally near the area of compression. This means the amount of possible drawing force is limited by the tensile strength of the material, a fact that is particularly evident when drawing thin wires.
The starting point of cold drawing is hot-rolled stock of a suitable size.
Processes.
Metal.
Sheet metal.
The success of forming is in relation to two things, the flow and stretch of material. As a die forms a shape from a flat sheet of metal, there is a need for the material to move into the shape of the die. The flow of material is controlled through pressure applied to the blank and lubrication applied to the die or the blank. If the form moves too easily, wrinkles will occur in the part. To correct this, more pressure or less lubrication is applied to the blank to limit the flow of material and cause the material to stretch or set thin. If too much pressure is applied, the part will become too thin and break. Drawing metal requires finding the correct balance between wrinkles and breaking to achieve a successful part.
Deep drawing and shallow drawing.
Sheet metal drawing becomes "deep drawing" when the workpiece is drawing longer than its diameter. It is common that the workpiece is also processed using other forming processes, such as piercing, ironing, necking, rolling, and beading.
In "shallow drawing", the depth of drawing is less than the smallest dimension of the hole.
Bar, tube, and wire.
Bar, tube, and wire drawing all work upon the same principle: the starting stock drawn through a die to reduce the diameter and increase the length. Usually the die is mounted on a draw bench. The end of the workpiece is reduced or pointed to get the end through the die. The end is then placed in grips and the rest of the workpiece is pulled through the die. Steels, copper alloys, and aluminium alloys are common materials that are drawn.
Drawing can also be used to cold-form a shaped cross-section. Cold drawn cross-sections are more precise and have a better surface finish than hot extruded parts. Inexpensive materials can be used instead of expensive alloys for strength requirements, due to work hardening.
Bar drawing.
Bars or rods that are drawn cannot be coiled therefore straight-pull draw benches are used. Chain drives are used to draw workpieces up to . Hydraulic cylinders are used for shorter length workpieces.
The reduction in area is usually restricted to between 20 and 50%, because greater reductions would exceed the tensile strength of the material, depending on its ductility. To achieve a certain size or shape multiple passes through progressively smaller dies or intermediate anneals may be required.
Tube drawing.
Tube drawing is very similar to bar drawing, except the beginning stock is a tube. It is used to decrease the diameter, improve surface finish and improve dimensional accuracy. A mandrel may or may not be used depending on the specific process used. A floating plug may also be inserted into the inside diameter of the tube to control the wall thickness.
Wire drawing.
This technique has long been used to produce flexible metal wire by drawing the material through a series of dies of decreasing size. These dies are manufactured from a number of materials, the most common being tungsten carbide and diamond.
Glass.
Similar drawing processes are applied in glassblowing and in making glass and plastic optical fiber.
Plastics.
Plastic drawing, sometimes referred to as "cold drawing", is the same process as used on metal bars, but applied to plastics.
Plastic drawing is primarily used in manufacturing plastic fibers. The process was discovered by Julian W. Hill (1904–1996) in 1930 while trying to make fibers from an early polyester. It is performed after the material has been "spun" into filaments; by extruding the polymer melt through pores of a spinneret. During this process, the individual polymer chains tend to somewhat align because of viscous flow. These filaments still have an amorphous structure, so they are drawn to align the fibers further, thus increasing crystallinity, tensile strength, and stiffness. This is done on a draw twister machine.
For nylon, the fiber is stretched to four times its spun length. The crystals formed during drawing are held together by hydrogen bonds between the amide hydrogens of one chain and the carbonyl oxygens of another chain.
Polyethylene terephthalate (PET) sheet is drawn in two dimensions to make BoPET (biaxially-oriented polyethylene terephthalate) with improved mechanical properties.